Abstract
We address the longstanding problem of the microscopic origin of the richly diverse phenomena in the chromium breathing pyrochlore material family. Combining electronic structure and renormalization group techniques we resolve the magnetic interactions and analyze their reciprocalspace susceptibility. We show that the physics of these materials is principally governed by longrange Heisenberg Hamiltonian interactions, a hitherto unappreciated fact. Our calculations uncover that in these isostructural compounds, the choice of chalcogen triggers a proximity of the materials to classical spin liquids featuring degenerate manifolds of wavevectors of different dimensions: A Coulomb phase with threedimensional degeneracy for LiInCr_{4}O_{8} and LiGaCr_{4}O_{8}, a spiral spin liquid with twodimensional degeneracy for CuInCr_{4}Se_{8} and onedimensional line degeneracies characteristic of the facecentered cubic antiferromagnet for LiInCr_{4}S_{8}, LiGaCr_{4}S_{8}, and CuInCr_{4}S_{8}. The surprisingly complex array of prototypical pyrochlore behaviors we discovered in chromium spinels may inspire studies of transition paths between different semiclassical spin liquids by doping or pressure.
Introduction
Over the past 30 years, materials with magnetic moments on the vertices of networks of cornershared triangular or tetrahedral units have played center stage in the experimental search for exotic magnetic states driven by competing, i.e. frustrated, interactions.^{1} In this context, the pyrochlore lattice of cornershared tetrahedra has emerged as a quintessential example of high frustration in three dimensions with a multitude of new phenomena having been uncovered.^{2}
In particular, for rareearth pyrochlore oxides with a trivalent \(4f\) magnetic ion, there is a wealth of stoichiometric compounds available in large singlecrystal form, necessary for detailed neutron scattering studies. This, along with the synergetic dialog between theory and experiments, has led to the experimental discovery and the theoretical rationalization of numerous phenomena like spin ice physics, magnetic moment fragmentation, orderbydisorder, fragile splayedferromagnetism and candidate spin liquid phenomenology.^{3,4}
In contrast with the above rareearth systems characterized by strongly anisotropic interactions at the \(O(1)\) K scale, there is a paucity of magnetic compounds involving transition metal ions on a pyrochlore network and coupled via a primarily isotropic Heisenberg exchange of a high (\(O(1{0}^{2})\) K) energy scale. The availability of such compounds in singlecrystal form would empower researchers to explore and possibly discover novel collective behaviors existing over a wider and more experimentally accessible temperature window. Specifically, this would allow exposing new ways in which perturbations, which might have appeared inconsequential from a cursory assessment, ultimately emerge as the dictating forces behind the lowtemperature and lowenergy scale physics of the material. In that regard, the recent successful synthesis of magnetic pyrochlore fluorides \(AB{M}_{2}\)F_{7} (\(A=\) Na; \(B=\) Ca, Sr; \(M=\) Ni, Co, Fe, Mn) in large single crystals is indeed an exciting and most welcome development in the field of highly frustrated magnetism.^{5} There is, however, a shortcoming with the latter compounds whose implications remain to be fully ascertained: The cation disorder on the nonmagnetic \(A\) and \(B\) sites is expected to randomize the \(M\)\(M\) superexchange and, most likely, ultimately drive the lowtemperature state of these systems to a semiclassical spin glass phase, albeit with some nontrivial spin dynamics.^{5} In this context, the disorderfree socalled breathing chromium spinels, which define a fairly broad range of materials (e.g. LiInCr_{4}O_{8}, LiGaCr_{4}O_{8}, LiInCr_{4}S_{8}, LiGaCr_{4}S_{8}, CuInCr_{4}S_{8}, and CuInCr_{4}Se_{8}),^{6,7,8,9,10,11,12,13,14,15,16} constitute a significant opportunity for carrying out the above research program in and below the \(O(1{0}^{2})\) K temperature scale.
The introduction of a breathing degree of freedom to the regular pyrochlore lattice, characterized by the alternation of small and large tetrahedra, results in two inequivalent nearestneighbor exchange couplings, with \(J\) for the small and \(J^{\prime}\) for the large tetrahedron, and adds a new level of complexity and thus richness to the regular pyrochlore Heisenberg Hamiltonian.^{1} In the breathing chromium spinels, of chemical formula \(AA^{\prime}\)Cr_{4}X_{8} (\(A\) = Li, Cu; \(A^{\prime}\) = Ga, In; \(X\) = O, S, Se), the magnetic Cr^{3+} spin \(S=3/2\) resides on a breathing pyrochlore lattice (see Fig. 1). Of particular interest, thanks to their significantly different size, the ions at the \(A\) and \(A^{\prime}\) sites do not chemically admix (i.e. they order), and the breathing chromium spinels are not subject to the \(A/B\) site disorder and consequential exchange randomness of the aforementioned \(AB{M}_{2}\)F_{7} pyrochlores. While an ordered arrangement of the \(A\) and \(A^{\prime}\) cations was first reported over halfacentury ago,^{17} it is only recently that breathing chromium spinels have become a subject of focused attention.^{6} A variety of experimental results have been reported, including a complex sequence of structural and magnetic transitions in LiInCr_{4}O_{8} and LiGaCr_{4}O_{8},^{8,9,11,12} as well as a halfmagnetization plateau in high magnetic field measurements on LiInCr_{4}O_{8}.^{13}
On the theoretical front, the properties of the classical nearestneighbor breathing pyrochlore Hamiltonian have been investigated,^{18} and spin–spin correlations in the ground state^{19} and the effects of spin–lattice coupling^{20} have been explored. Possible implications of the topological aspects of magnetic excitations in the breathing pyrochlore lattice have been pointed out.^{21,22} However, to the best of our knowledge, there appears to have been no attempt to (i) provide a microscopic determination of the Cr–Cr exchange interactions and to (ii) investigate using an unbiased theoretical framework the implications of the concurrent thermal and quantum fluctuations operating in these compounds. Such an endeavor is necessary to gain a deeper microscopic understanding of the already available experimental results beyond the simplest interpretation currently provided, as well as identifying new and exciting avenues of investigation in these materials—this is the purpose of the present work. As we shall discuss later on, different signs (ferromagnetic or antiferromagnetic) exchange couplings \(J\) and \(J^{\prime}\) are realized in the oxides (\(X=\) O), sulfide (\(X=\) S) and selenides (\(X=\) Se) breathing chromium spinels. This provides an uncharted territory for the investigation of the nontrivial role played by longrange interactions beyond \(J\) and \(J^{\prime}\) in these materials. This leads us to propose that breathing chromium spinels constitute a promising platform to explore the role of strong competing longrange interactions in a semiclassical (\(S=3/2\)) regime. In particular, we predict these to engender new forms of nontrivial correlations in the cooperative paramagnetic regime characterized by different classically degenerate ground state manifolds of different dimension and intricate magnetic orders at low temperatures. Examples include emergent effective Heisenberg antiferromagnetism on the facecentered cubic lattice,^{18} a Coulomb phase,^{23} and a spiral spin liquid.^{24}
Results
Breathing pyrochlore Hamiltonians
Room temperature structures
We first perform electronic structure calculations for all presently known room temperature structures of chromium breathing spinels. We use the structures of Okamoto et al.^{6} for LiInCr_{4}O_{8} and LiGaCr_{4}O_{8}, the structures of Okamoto et al.^{16} for LiInCr_{4}S_{8}, LiGaCr_{4}S_{8}, and CuInCr\({}_{4}\)S\({}_{8}\) and that of Duda et al.^{7} for CuInCr_{4}Se_{8}. The main exchange connectivity of all structures is illustrated in Fig. 1. We follow the experimental literature^{6,8,9,11} in referring to the exchange couplings within the small and large tetrahedra as \(J\) and \(J^{\prime}\), respectively. As in the isotropic pyrochlore lattice,^{25} there are 12 second nearest neighbors \({J}_{2}\) and 12 third nearest neighbors which split into two symmetry inequivalent classes; six of these, named \({J}_{3a}\), have an inbetween Cr^{3+} ion, and the six others, named \({J}_{3b}\), do not.
Figure 2 presents the first main result of our work. The exchange couplings as defined in the Heisenberg Hamiltonian of the form
are shown as a function of interaction strength \(U\) in the GGA+\(U\) functional. For all six compounds, a unique \(U\) value can be determined at which the couplings yield the experimental Curie–Weiss temperature (vertical lines). These fixed parameter values lead to the sets of Hamiltonian couplings given in Table 1. The \(U\) values are very reasonable^{26} for Cr^{3+} and are all located in a narrow interval \(1.43\ \,\text{eV}\,\le U\le 1.91\ \,\text{eV}\,\), indicating that the great diversity among the chromium breathing pyrochlores, varying from antiferromagnetic to ferromagnetic Heisenberg models, can all be described with roughly the same exchange correlation functional. We find that both oxides, LiInCr_{4}O_{8} and LiGaCr_{4}O_{8}, are dominated by antiferromagnetic \(J\) and \(J^{\prime}\) couplings (Fig. 2a, b), with longer range couplings being very small. Interestingly, it is found that in LiGaCr_{4}O_{8} the large tetrahedron is associated with the larger exchange coupling. The calculated breathing exchange anisotropy for LiGaCr_{4}O_{8} is \({B}_{\mathrm {{f}}}\equiv J/J^{\prime} =0.66\), very close to the experimental estimate \({B}_{\mathrm {{f}}}=0.6\).^{6} However, according to our calculation, LiInCr_{4}O_{8} at \({B}_{\mathrm {{f}}}\equiv J^{\prime} /J=0.37\) is far less anisotropic than assumed so far (\({B}_{\mathrm {{f}}}=0.1\)).^{6} For the sulfides LiInCr_{4}S_{8}, LiGaCr_{4}S_{8}, and CuInCr_{4}S_{8} (Fig. 2d–f), the large tetrahedron is characterized by ferromagnetic exchange \(J^{\prime}\). However, the biggest surprise here is the presence of substantial secondneighbor and thirdneighbor couplings. As each Cr^{3+} ion has a total of 24 such bonds, compared to six \(J\) or \(J^{\prime}\) bonds, they can have a substantial influence on the behavior of the materials. Interestingly, the fact that the experimentally determined Curie–Weiss temperature of LiGaCr_{4}S_{8} is small is thus readily explained by a cancellation of ferromagnetic \(J\) and \(J^{\prime}\) by antiferromagnetic \({J}_{2}\) and \({J}_{3a}\), \({J}_{3b}\) couplings rather than by opposite signs of \(J\) and \(J^{\prime}\) as hypothesized in ref. ^{16}. Opposite signs of \(J\) and \(J^{\prime}\) are only found for CuInCr_{4}S_{8}. Finally, the selenide CuInCr_{4}Se_{8} (Fig. 2c) is dominated by ferromagnetic \(J\) and \(J^{\prime}\) couplings; however, even for this compound, the third neighbor couplings \({J}_{3a}\) and \({J}_{3b}\) are antiferromagnetic and, most importantly, nonnegligible.
Temperature dependence
For most materials, only a room temperature structure is on record. However, ref. ^{9} gives a \(T=20\) K structure for LiInCr_{4}O_{8}, while Pokharel et al.^{15} provide a \(T=10\) K structure for LiGaCr_{4}S_{8}. The two Cr–Cr distances within small and large tetrahedra for these two structures are tabulated along with the measurements of the six room temperature structures in Supplementary Table 2. While the (structural) breathing anisotropy of the oxide LiInCr_{4}O_{8} decreases significantly at low temperature, it is essentially temperature independent for the sulfide LiGaCr_{4}S_{8}. Studying the two cubic lowtemperature structures can give us an indication of how temperature dependent the electronic behavior of the breathing pyrochlore materials is within the cubic \(F\bar{4}3m\) structure. Clearly, a systematic study of the temperature dependence of the exchange couplings would require more detailed structural information for the other materials. The last two lines of Table 1 show the exchange interactions calculated for the two lowtemperature structures. Even though the lowtemperature structure of LiInCr\({}_{4}\)O\({}_{8}\) has a reduced breathing anisotropy of \(r^{\prime} /r=1.029\), compared to \(r^{\prime} /r=1.051\) at room temperature, the exchange couplings \(J\) and \(J^{\prime}\) become nearly identical (see Supplementary Fig. 1), with the room temperature exchange anisotropy of \(J^{\prime} /J=0.37\) having been eliminated. For LiGaCr\({}_{4}\)S\({}_{8}\), while the low temperature structural anisotropy is still significant at \(r^{\prime} /r=1.070\), the two ferromagnetic couplings \(J\) and \(J^{\prime}\) become very similar near the \(U\) value determined by the experimental \({\theta }_{{\rm{CW}}}\) (see Supplementary Fig. 1). Thus, we find that the nearestneighbor exchanges \(J\) and \(J^{\prime}\) remain antiferromagnetic for LiInCr_{4}O_{8} and ferromagnetic for LiGaCr_{4}S_{8}, but in both cases they become very similar at low temperatures. At the same time, the further neighbor couplings remain very small for the oxide and substantial for the sulfide.
Energy mapping clearly identifies three different types of breathing pyrochlore Hamiltonians: Mostly antiferromagnetic oxides, sulfides with ferromagnetic large tetrahedron and antiferromagnetic longer range \(({J}_{2},{J}_{3{\rm{a}}},{J}_{3{\rm{b}}})\) exchange, and the mostly ferromagnetic selenide perturbed by crucial antiferromagnetic longer range interactions. Thus, we organize our pseudofermion functional renormalization group (FRG) analysis of the Hamiltonians into oxide, sulfide, and selenide sections.
Pseudofermion FRG calculations
Oxides
For LiInCr_{4}O_{8} and LiGaCr_{4}O_{8}, the \(J\) and \(J^{\prime}\) couplings forming the tetrahedra are both antiferromagnetic. With only these two couplings, one would expect the typical bowtie features with the associated pinch points in the reciprocal space susceptibility at sufficiently low temperatures (see ref. ^{27}). In this previous study, we showed that the inclusion of even very weak second nearestneighbor couplings can dramatically alter the susceptibility profile of the nearestneighbor ground state phase and destroy the pinch points and bowties.^{28} As stated above, for both breathing pyrochlore oxides, our DFT analysis reveals the presence of additional antiferromagnetic \({J}_{2}\), \({J}_{3a}\), and \({J}_{3b}\) couplings (see Table 1). At the classical level, it is known that when the dominant interactions \(J\) and \(J^{\prime}\) are large and antiferromagnetic such that the four spins at the vertices of each tetrahedron can be assumed to sum to zero approximately, then a third neighbor coupling \({J}_{3a}\) in an ideal pyrochlore lattice is equivalent at temperature \(T\ll \min (J/{k}_{{\rm{B}}},J^{\prime} /{k}_{{\rm{B}}})\) to a \({J}_{2}\) coupling of opposite sign.^{28,29} Thus, effectively, both chromium oxides are approximately described by a pyrochlore Hamiltonian with antiferromagnetic \(J\), \(J^{\prime}\) and ferromagnetic \({J}_{2}\): \(({J}_{2}{J}_{3a})/\bar{J}=0.025\) for LiInCr\({}_{4}\)O\({}_{8}\) and \(0.011\) for LiGaCr\({}_{4}\)O\({}_{8}\) (\(\bar{J}=\sqrt{{J}^{2}+J{^{\prime} }^{2}}\) is the overall nearestneighbor energy scale, listed in Supplementary Table 1). According to ref. ^{27}, we expect that the spectral weight moves away from the pinch point and forms two symmetrical maxima, resulting in a hexagonal cluster pattern of intensities in the \([hhl]\) plane. Indeed, using the exchange couplings obtained for the room temperature structure (see Table 1), we employ PFFRG to calculate the magnetic susceptibility profiles which are shown in Fig. 3a, b, d, e. They are found to closely resemble the susceptibility of the isotropic \({J}_{1}\)−\({J}_{2}\) pyrochlore magnet for antiferromagnetic \({J}_{1}\) and ferromagnetic \({J}_{2}\).^{27} It is worth noting that, due to the relatively weaker effective second nearestneighbor coupling in LiGaCr_{4}O_{8}, the pinch points and bowties are better preserved at low temperature for LiGaCr_{4}O_{8} (see Fig. 3d) in comparison to LiInCr_{4}O_{8} (Fig. 3a). However, from our PFFRG calculations we find that for both oxides, and at all temperatures down till the RG flow breakdown, the maxima of the susceptibility are always located at the highsymmetry \(W\) point in the extended Brillouin zone, i.e., at a \({\bf{q}}=\frac{2\pi }{a}(2,1,0)\)type ordering vector (see Supplementary Note 2), as found in ref. ^{27} for the nearestneighbor isotropic \(S=3/2\) Heisenberg antiferromagnet. A direct space schematic illustration for the spin configuration corresponding to this order is shown in Fig. 4a. In direct space, for this spin configuration, the pyrochlore lattice decomposes into two pairs of fcc sublattices. Within each pair, the two fcc sublattices are separated from each other by a nearestneighbor vector which is perpendicular to the \(\frac{2\pi }{a}\) component of the ordering vector, e.g., for a \(\frac{2\pi }{a}(2,1,0)\)ordering vector, one pair of fcc sublattices is separated by the vector \(\frac{a}{4}(1,0,1)\) and the other pair is separated by the vector \(\frac{a}{4}(1,0,1)\). All fcc sublattices show a stripe antiferromagnetic order, i.e., spins are antiferromagnetically aligned in the \(\frac{2\pi }{a}\)direction and ferromagnetically in the perpendicular directions. Within each pair, the neighboring spins of different sublattices are aligned antiparallel in spin space. The two pairs can be rotated freely with respect to each other. In reciprocal space, this configuration leads to main Bragg peaks at all \(\frac{2\pi }{a}(2,1,0)\)type vectors which share the same \(\frac{2\pi }{a}\) component, e.g., \(\frac{2\pi }{a}(2,1,0)\), \(\frac{2\pi }{a}(2,1,0)\), \(\frac{2\pi }{a}(0,1,2)\), \(\frac{2\pi }{a}(0,1,2)\), \(\frac{2\pi }{a}(2,1,0)\), \(\frac{2\pi }{a}(2,1,0)\), \(\frac{2\pi }{a}(0,1,2)\), and \(\frac{2\pi }{a}(0,1,2)\). In the reciprocal plane perpendicular to the \(\frac{2\pi }{a}\)direction, the relative orientation of the sublattices results in subdominant Bragg peaks with half the intensity of the dominant ones at the \(\frac{2\pi }{a}(1,0,1)\)type vectors in this plane, i.e., at \(\frac{2\pi }{a}(1,0,1)\), \(\frac{2\pi }{a}(1,0,1)\), \(\frac{2\pi }{a}(1,0,1)\), \(\frac{2\pi }{a}(1,0,1)\). For the classical model of LiGaCr_{4}O_{8}, this state is the exact ground state given by the Luttinger–Tisza method and confirmed with the iterative minimization procedure. However, we find that this state is strongly dependent on the interplay between the two kinds of third nearestneighbor couplings. This leads to the finding that for LiInCr_{4}O_{8}, due to the larger difference between \({J}_{3a}\) and \({J}_{3b}\), an incommensurate order on the sublattices is stabilized as the ground state found by iterative minimization. We would like to emphasize that the stabilization of the orders discussed above rests crucially on the presence and the relative magnitude of the third nearestneighbor couplings. Indeed, classically, the pure \({J}_{1}\)\({J}_{2}\)model on a regular \({J}_{1}\equiv J=J^{\prime}\) pyrochlore lattice would feature a \({\bf{q}}={\bf{0}}\) state, completely different from the \(\frac{2\pi }{a}(2,1,0)\)order found here.
To make contact with experimental results, it is useful to assess the temperature dependence of the structure factor as calculated within PFFRG. The relation \(T=(2\pi /3)S(S+1)\Lambda\) can be used to relate the infrared cutoff \(\Lambda\) employed in the PFFRG framework to temperature \(T\).^{27,30} The relation is obtained by comparing the classical limit (\(S\to \infty\)) of PFFRG, where only the RPA diagrams contribute, i.e. a meanfield description, with the conventional spin meanfield theory formulated in terms of temperature \(T\) instead of \(\Lambda\). The resulting estimated ordering temperatures are given in Supplementary Note 2. As explained in detail in the Appendix A of ref. ^{27}, in the \(S\to \infty\) limit, the absence of higher diagrammatic orders in \(1/S\) in the oneloop PFFRG used here implies that, in particular for the nearestneighbor pyrochlore antiferromagnetic Heisenberg model, a spurious divergence of the susceptibility at finite temperature occurs which is not expected from what is well established for the classical problem.^{23,27} Thus, our estimates of the ordering temperatures in all of the pyrochlore magnets considered here are systematically too high.^{31} Our comparisons to an experimental temperature \(T\) are shown for a \(\Lambda\) obeying \(\Lambda /{\Lambda }_{{\rm{c}}}={T}^{\exp }/{T}_{{\rm{c}}}^{\exp }\). It is expected that multiloop implementations of PFFRG will lead to significant improvements for the calculated temperature scales;^{32,33} however, these advanced schemes are still under development.
We have also performed the PFFRG calculation for the LiInCr_{4}O_{8} Hamiltonian corresponding to its lowtemperature structure (see Table 1, last but one line). The calculated susceptibility profile (see Supplementary Fig. 4) is seen to be virtually indistinguishable from that obtained from the room temperature structure shown in Fig. 3a, b even though the breathing anisotropy of the Hamiltonian is significantly different, having evolved from \(J^{\prime} /J=0.37\) at room temperature to \(J^{\prime} /J\cong 1\) at \(T=20\) K. The general observation of the magnetic response being largely independent of the breathing anisotropy can be understood from a classical picture. As discussed in the Supplementary Note 3, the eigenvalues of the interaction matrix \({\mathcal{J}}({\bf{k}})\) for a \(J\)−\(J^{\prime}\)only model exhibit flat bands at the lowest energies which determine the typical bowtie features of pyrochlore antiferromagnets. Interestingly, these flat bands persist for any \(J\ >\ 0\) and \(J^{\prime}\ >\ 0\)^{18} (see Supplementary Fig. 7), rendering the momentum space profile of the magnetic susceptibility independent of \(J^{\prime} /J\). As a consequence, longer range \({J}_{2}\), \({J}_{3a}\), \({J}_{3b}\) have the opportunity to play a crucial role in determining the magnetic behavior of the system. In the present case, however, we find that the effective secondneighbor coupling of LiInCr_{4}O_{8} at 20 K given by \(({J}_{2}{J}_{3a})/\bar{J}=0.030\) is nearly unchanged compared to room temperature (see Supplementary Table 1) thus leading to almost identical magnetic responses.
It is now interesting to compare and verify the accuracy of the Hamiltonian determined for LiInCr_{4}O_{8} against polarized neutronscattering data from powder samples of Okamoto et al.^{10}. It was shown by Benton et al.^{18} that within the selfconsistent Gaussian approximation (SCGA), the experimental estimate \(J^{\prime} /J=0.1\), or even a range \(0.05\,\lesssim\, J^{\prime} /J\,\lesssim\, 0.15\), is consistent with the neutron data. We also calculate the product \( F(Q){ }^{2}S(Q)\) of the magnetic form factor \( F(Q){ }^{2}\) and the powder averaged structure factor \(S(Q)\) using
for all the materials considered here.^{34} The \(S(Q)\) is calculated using both the quantum \(S=3/2\) PFFRG and classical Monte Carlo (CMC) methods. We show in Fig. 5a, b the comparison to the \(T=30\) K and the \(T=150\) K neutronscattering data. The PFFRG calculations for the DFT determined Hamiltonians for LiInCr_{4}O_{8} at room temperature (\(J^{\prime} /J=0.37\)) as well as at \(T=20\) K (\(J^{\prime} /J=1\)), upon inclusion of the secondneighbor and thirdneighbor couplings, give an excellent agreement with the \(T=30\) K neutron data. In contrast, the CMC results, both for the room temperature as well as \(T=20\) K couplings, progressively lose agreement as \(Q\) is lowered. This observation may hint towards the nonnegligible role of quantum fluctuations in accurately capturing the correlations especially at low \(Q\) values. The excellent agreement of the earlier SCGA calculations of ref. ^{18} is also likely rooted in the fact that in this approach the “hard constraint”, namely, that the spin vector on each site has magnitude \(S\), is relaxed and only implemented on average. This may tacitly incorporate some effects of quantum fluctuations by allowing for fluctuations of the classical moments.^{35} At \(T=150\) K, the neutron data essentially follows the \(Q\) dependence of the magnetic form factor;^{10} while the computed scattering intensities for the room temperature and \(T=20\) K Hamiltonians are consistent, the agreement with the experimental \(T=150\) K neutron data is neither satisfactory for the PFFRG nor for the CMC results. A similar observation has already been made by Benton et al.^{18} and thus remains unexplained (see also Supplementary Note 2).
Sulfides
We have performed PFFRG calculations for all three chromium sulfides, LiInCr_{4}S_{8}, LiGaCr_{4}S_{8} and CuInCr_{4}S_{8}. As we find very similar susceptibility profiles for the three compounds, we show the one for CuInCr_{4}S_{8} in Fig. 3g, h and the other two in Supplementary Fig. 4. CuInCr_{4}S_{8} has a ferromagnetic \(J^{\prime}\) which is the strongest among all the interactions present in this material. At the low temperatures that we are considering here, we can therefore assume that the four spins on the large tetrahedra point in approximately the same direction, thereby behaving as effective spin6 entities. Since the large tetrahedra are arranged in a face centered cubic (fcc) magnetic lattice (see Supplementary Fig. 5), the system can effectively be mapped onto a spin6 Heisenberg Hamiltonian on a fcc lattice with renormalized nearestneighbor couplings \({J}_{1}^{{\rm{fcc}}}=(J+4{J}_{2}+2{J}_{3a}+2{J}_{3b})/16\). These couplings are all antiferromagnetic with values \({J}_{1}^{{\rm{fcc}}}=1.11\) K for LiInCr_{4}S_{8}, \({J}_{1}^{{\rm{fcc}}}=0.95\) K for LiGaCr_{4}S_{8} and \({J}_{1}^{{\rm{fcc}}}=2.56\) K for CuInCr_{4}S_{8}. Interestingly, the nearestneighbor antiferromagnetic classical Heisenberg model on the fcc lattice features a subextensive (\({\mathcal{O}}[L]\)) ground state degeneracy in the classical limit (\(S\to \infty\)), with associated wave vectors of the form \({\bf{q}}=\frac{2\pi }{a}(1,\delta ,0)\) and symmetryrelated \({\bf{q}}\).^{36} This degeneracy appears as lines of strong intensity in the magnetic response. However, as further explained in Supplementary Note 5, the susceptibility profile of our pyrochlore model differs from that of the regular fcc antiferromagnet, since it is modulated by a form factor arising from the presence of a tetrahedral basis of our effective fcc lattice. For the structure factors in the \([hk0]\) plane, this leads to a square ringtype structure formed by lines of strong and almost constant intensity^{18} (see Fig. 3h and Supplementary Fig. 4). The point \({\bf{q}}=\frac{2\pi }{a}(1,0,0)\) (and symmetryrelated \({\bf{q}}\)space positions) is special because it resides at the junctions of the ground state manifold \({\bf{q}}=\frac{2\pi }{a}(1,\delta ,0)\) and \({\bf{q}}=\frac{2\pi }{a}(1,0,\delta )\). Because of this, it is found that collinear ordered states with the ordering wave vector of the type \({\bf{q}}=\frac{2\pi }{a}(1,0,0)\) are selected by thermal,^{36} as well as quantum^{37}orderbydisorder mechanism. As the PFFRG method incorporates the combined effects of thermal and quantum fluctuations, and thus of their selection effect, it is interesting to note that our analysis reveals maxima at \({\bf{q}}=\frac{2\pi }{a}(1,0,0)\) type positions for all three sulfides (see Supplementary Note 2). The corresponding direct space spin configuration is illustrated in Fig. 4b. The astonishing property that all sulfides show almost identical susceptibility profiles even though the ratio \(J/J^{\prime}\) varies significantly between the three compounds can be understood by considering the eigenvalues of the interaction matrix \({\mathcal{J}}({\bf{k}})\) for a pyrochlore system with \(J\ >\ 0\) and \(J^{\prime}\ <\ 0\). As shown in Supplementary Fig. 7, the lowest band exhibits linelike degeneracies, regardless of the size of \(J/J^{\prime}\), leading to a magnetic response which is largely independent of this ratio.^{18}
Plumier et al.^{38,39} studied CuInCr_{4}S_{8} using unpolarized neutrons. In order to compare our calculations to this experiment, we subtract the room temperature neutron spectra from the low temperature spectra in order to remove the background. In Fig. 5c, d, this data is compared to the calculated structure factor \(S(Q)\) weighted with the magnetic form factor \( F(Q){ }^{2}\) of Cr^{3+} ions, i.e., \( F(Q){ }^{2}S(Q)\). For the 40 K neutron data, the experiment matches well with our numerical data from PFFRG up to an arbitrary scale factor. At 85 K, while the peak positions match very well between theory and the experimental intensity profile, the intensity has some deviation at low \(Q\). This could be partly due to the uncertainty in the mapping of the flow parameter \(\Lambda\) to temperature. Since 85 K is about 2.4\({T}_{{\rm{c}}}\) for CuInCr_{4}S_{8}, the calculated structure factor is compared at 2.4\({\Lambda }_{{\rm{c}}}\). Nevertheless, the comparison of the spin–spin correlation profile to the available experimental information lends strong support to the validity of the Hamiltonian we determine for CuInCr_{4}S_{8}. We have verified that all subleading couplings \({J}_{2}\), \({J}_{3a}\) and \({J}_{3b}\) as given in Table 1 are necessary to ensure this level of agreement with experiment; dropping any of them substantially deteriorates the comparison (Supplementary Fig. 6). On the other hand, CMC calculations are unable to capture the dominant correlations present in the 40 K experimental data, possibly hinting at the role of quantum fluctuations in accurately capturing the important correlations at low temperature, similar to what we observe in LiInCr_{4}O_{8}.
Selenide
The material CuInCr_{4}Se_{8} is the only selenide breathing chromium spinel with detailed structure reported for which we can perform calculations. At a first glance, the Hamiltonian parameters (Table 1) appear similar to those for LiGaCr_{4}S_{8}, with a ferromagnetic large tetrahedron. However, the PFFRG result shown in Fig. 3j–l displays a completely different spin susceptibility. In contrast to a repetition of the broken high intensity lines representative of the onedimensional subextensive degeneracy that we discussed in the previous subsection, we find the twodimensional degeneracy of a sphere in reciprocal space. The ferromagnetic large tetrahedra characterized by the \(J^{\prime}\) coupling form a large (\(S=6\)) moment fcc lattice with an effective nearestneighbor interaction given by \({J}_{1}^{{\rm{fcc}}}=(J+4{J}_{2}+2{J}_{3a}+2{J}_{3b})/16\) which evaluates to \({J}_{1}^{{\rm{fcc}}}=0.55\) K. The ferromagnetic nature of \({J}_{1}^{{\rm{fcc}}}\) in the selenide is indicative of the crucial difference between the selenide and the sulfides (for which the \({J}_{1}^{{\rm{fcc}}}\) are antiferromagnetic): in contrast to the sulfides, nearly negligible \({J}_{2}\) and smaller \({J}_{3a}\) and \({J}_{3b}\) couplings do not fully compensate the substantial ferromagnetic \(J\) anymore. Nonetheless, clearly no simple ferromagnetic order is realized in CuInCr_{4}Se_{8}. Rather, the two thirdneighbor couplings (taken together) substantially perturb the FM large tetrahedra, which leads to the appearance of a twodimensional degeneracy of classical ground states. At the ordering temperature (Supplementary Note 2), the system develops an incommensurate spiral magnetic order with a helix pitch vector \({\bf{q}}\approx \frac{2\pi }{a}(0.521,0,0)\) (and symmetryrelated points \((0,q,0)\) and \((0,0,q)\)). The corresponding magnetic susceptibility profile obtained from PFFRG at the ordering temperature is shown in Fig. 3j–k, wherein one observes peaks in \(S({\bf{q}})\) at \({\bf{q}}\,\ne\, {\bf{0}}\). The corresponding direct space spin configuration is illustrated in Fig. 4c. It is worth emphasizing that the shift of the spectral weight away from \({\bf{q}}={\bf{0}}\) is the combined effect of both \({J}_{3a}\) and \({J}_{3b}\) couplings of a comparable magnitude.^{40} Above the ordering temperature, and within the cooperative paramagnetic regime, we observe that the spectral weight is distributed rather uniformly over the spiral surface suggesting the presence of an approximate spiral spin liquid on the pyrochlore lattice stabilized concomitantly by thermal and quantum fluctuations. While an incommensurate longrange ordered spiral phase of \((q,0,0)\) type has been observed for the material ZnCr_{2}Se_{4} with pyrochlore magnetic lattice,^{40} it is only very recently that a spiral spin liquid has been observed in the chromium spinel MgCr_{2}O_{4}.^{41}
The spin spiral surface found in the cooperative paramagnetic regime in a PFFRG calculation, is also found to be present in the corresponding classical model at \(T=0\), as revealed by a Luttinger–Tisza analysis. However, the Luttinger–Tisza eigenstates on this spiral surface generically do not represent real normalizable spin configurations, i.e., the spin length on different fcc sublattices are not equal in magnitude. It turns out that, it is only for the \((q,0,0)\)type ordering vectors (with \({\bf{q}}\approx \frac{2\pi }{a}(0.45,0,0)\)) that the minimal energy can be achieved by a configuration of normalized spins. This ground state configuration then breaks the symmetry of the lattice as it is only governed by one of the three \((q,0,0)\)type vectors. Indeed, our CMC calculations give an ordering vector of \({\bf{q}}=\frac{2\pi }{a}(0.40\pm 0.04,0,0)\) at the transition temperature. Although the spiral surface is inaccessible at \(T=0\) due to the violation of the spin length constraint, thanks to thermal and/or quantum fluctuations it can in principle be made accessible. Indeed, for CuInCr_{4}Se_{8}, our PFFRG analysis shows that thermal and quantum fluctuations taken together are able to restore a welldefined spin spiral surface (see Fig. 3j, k) right above the ordering temperature. In contrast, our CMC simulations, right above the ordering temperature, find a highly nonuniform distribution of spectral weight, and thus an absence of spiral spin liquid, however, as the temperature is increased to \(\sim 1.5\) times the ordering temperature, a spiral surface appears (compare Supplementary Fig. 8 with Fig. 3j, k above). These findings lend support to the role played by quantum fluctuations in aiding the stabilization of a spiral spin liquid. It is worth noting that within the ordered phase, this single\({\bf{q}}\) state does not however represent a single planar spiral throughout the entire lattice. Instead, similar to what is found in CuInCr_{4}S_{8}, the lattice can be divided into two pairs of fcc sublattices. Within each pair, the sublattices are connected by a nearestneighbor vector perpendicular to the ordering vector, and the planar spiral orders within each pair are of equal pitch and phase. However, the two pairs of fcc sublattices are found to be out of phase with respect to each other by ~\({5}^{\circ }\). This offset in phase is a direct and unique consequence of the breathing anisotropy, and is found to vanish in the isotropic pyrochlore lattice.
Discussion
One of the important findings of this study is the significant and heretofore unappreciated role played by longrange exchange interactions on the breathing pyrochlore lattice. While we have previously pointed out the sensitivity of the spin structure factor to the sign and size of the subleading couplings in the \({J}_{1}\)−\({J}_{2}\) quantum pyrochlore Heisenberg antiferromagnet,^{27} we have found in the present work for the chromium breathing pyrochlores an impressive demonstration of the decisive role played by longerrange couplings, i.e., the two kinds of symmetry inequivalent thirdnearestneighbor couplings \({J}_{3a}\) and \({J}_{3b}\). On the other hand, the effects of breathing anisotropy are shown to be surprisingly minor. Indeed, we observe that in LiInCr_{4}O_{8}, the effective ferromagnetic secondneighbor coupling of 2.5% of the average nearestneighbor coupling far outweighs the substantial room temperature breathing anisotropy of \(J^{\prime} /J=0.37\) in its effect on the structure factor profile. In the case of the sulfides, although the \(J^{\prime} /J\) ratios vary between 93 and \(1.8\) among the three compounds, the susceptibility profiles appear all very similar. In this case, this is rooted in the effective mapping of the system to an emerging effective nearestneighbor fcc Heisenberg antiferromagnet with the fcc lattice sites being occupied by ferromagnetic tetrahedra featuring a large \(S=6\) magnetic moment. In this case, we show that the spin structure factor displays linelike degeneracies which are, once more, largely independent of the breathing anisotropy ratio \(J^{\prime} /J\). Finally, for the dominantly ferromagnetic selenide CuInCr_{4}Se_{8}, we demonstrate that the combined effect of the two thirdneighbor couplings \({J}_{3a}\) and \({J}_{3b}\) drastically perturbs the ground state away from the simple ferromagnetic order. Interestingly, we find that the perturbed state corresponds to an approximate spiral spin liquid above the ordering temperature and within the cooperative paramagnetic regime, where the individual wave vectors form a spherelike manifold in reciprocal space. Our PFFRG analysis indicates that the combined effect of quantum and thermal fluctuations only leads to a weak orderbydisorder selection into an incommensurate spiral state. Approximate spiral spin liquids on threedimensional lattices are so far known only on the diamond lattice in MnSc_{2}S_{4},^{24,31,42} with an occurrence having also been very recently reported for the pyrochlore material MgCr_{2}O_{4}.^{41}
We have theoretically investigated six chromium spinels featuring crystalline, and thus magnetic exchange breathing anisotropy. The Hamiltonians which were determined from density functional theory calculations and investigated using the pseudofermion FRG method showcase a colorful selection of magnetic properties arising from frustrated interactions. We find that the oxide compounds are in a perturbed Coulomb phase,^{23} reminiscent of the famous spin ice materials. The sulfides display an effective fcc lattice Heisenberg antiferromagnetictype behavior, and the selenide features incommensurate magnetic correlations. As a unifying feature, all materials are found to be close to a classical degeneracy which shows up as different variants: The oxides are near a phase featuring an extensive number of classical ground states scaling exponentially in the volume of the system. The selenide is approximately degenerate on a twodimensional surface with a manifold of states scaling exponentially in \({L}^{2}\) (where \(L\) is the linear dimension of the system). Finally, the sulfides are characterized by approximate linelike degeneracies with the number of ground states scaling exponentially in the linear dimension \(L\). This variety of different behaviors in a family of related materials represents an attractive feature which promises a wealth of opportunity for future investigations; on the one hand, doping series interpolating between different types of ground states could be very interesting. On the other, it is an intriguing question how other known but only sketchily characterized breathing chromium spinels like CuGaCr_{4}S_{8}, AgInCr_{4}S_{8}, CuGaCr_{4}Se_{8}, AgInCr_{4}Se_{8}^{43} fit the picture outlined in this study. Of particular importance are experimental investigations with single crystals which would allow to assess our theoretical predictions.
Methods
Energy mapping method
We determine the electronic structure and total energies of the breathing pyrochlores using the full potential local orbital (FPLO) basis set^{44} and the generalized gradient approximation (GGA) functional.^{45} The GGA+\(U\)^{46} correction to the exchange and correlation functional is used to deal with the strong electronic correlations on the Cr\({}^{3+}\)\(3d\) orbitals. Two parameters enter these calculations, the onsite interaction strength \(U\) and the Hund’s rule coupling \({J}_{{\rm{H}}}\). As the Hund’s rule coupling is an intraatomic interaction, we do not expect it to vary much from one compound to the other, and thus henceforth fix its value to \({J}_{{\rm{H}}}=0.72\) eV as commonly employed for Cr^{3+}.^{47} Meanwhile, the onsite interaction \(U\) was fitted from the experimentally determined Curie–Weiss temperatures as explained below. Heisenberg Hamiltonian parameters are extracted using the energy mapping approach:^{31,48,49,50} For this purpose, a \(3\, \times 1\times 1\) supercell of the primitive unit of the cubic \(F\bar{4}3m\) structure with \(Cm\) space group is constructed. In this structure, there are 9 independent spins (out of 12 in total), allowing 75 spin configurations with different energies. Total energies are converged using \(6\,\times\, 6\,\times\, 6\, {\bf{k}}\) points. An arbitrary subset of 19 spin configurations allows us to fit six exchange interactions, using a Heisenberg Hamiltonian of the form of Eq. (1). Note that we count every bond only once. The quality of the fit is seen to be excellent (see Supplementary Fig. 2 for an example), indicating that the method works extremely well for the chromium breathing pyrochlores, may they be dominantly antiferromagnetic or ferromagnetic. Now, the \(U\) parameter of the GGA+\(U\) functional can be fixed: We calculate the Hamiltonian parameters for a small set of \(U\) values, which we choose such that the Curie–Weiss temperatures \({\theta }_{{\rm{CW}}}=\frac{1}{3}S(S+1)(3J+3J^{\prime} +12{J}_{2}+6{J}_{3a}+6{J}_{3b})\) (see Fig. 1) calculated from these Hamiltonians cover a range of temperatures which includes the experimental \({\theta }_{{\rm{CW}}}\). We find the \(U\) value from the condition \({\theta }_{{\rm{CW}}}^{{\rm{theor}}}={\theta }_{{\rm{CW}}}^{\exp }\) by interpolation (see Fig. 2). For the breathing pyrochlores, we find the \({\theta }_{{\rm{CW}}}^{{\rm{theor}}}\) to be monotonous functions of \(U\) and thus to allow for a unique solution. Some more discussion on \({\theta }_{{\rm{CW}}}\) and \(U\) can be found in Supplementary Note 1.
Pseudofermion FRG method
In the PFFRG scheme,^{51} a general spin\(S\) Heisenberg Hamiltonian, e.g. Eq. (1), is treated by first reexpressing the spin operator at each lattice site by \(2S\) spin1/2 degrees of freedom using Abrikosov pseudofermions. Aside from the desired Hilbert space of spin\(S\) states this approach also introduces unphysical states with lower spin magnitudes. Since these states contribute less to the energy of the system compared to the physical ones, they act as excitations and, thus, naturally get excluded at low temperatures in the RG process.^{27} Next, the pseudofermionic Hamiltonian is treated using the FRG formalism.^{51,52,53,54} Here, the bare fermionic Green’s function in Matsubara space is equipped with an infrared frequency cutoff \(\Lambda\) suppressing the fermionic propagation at low frequencies. The PFFRG flow equations then follow from the \(\Lambda\) dependence of the \(m\)particle irreducible vertex functions which are given by an exact and infinite hierarchy of coupled integrodifferential flow equations.^{52} For a numerical implementation, this hierarchy however needs to be truncated, which is done by neglecting threeparticle and higher vertex functions. Still, and most importantly, the truncated version of the method exactly sums up the full set of fermionic Feynman diagrams in two limits taken separately, namely, the large\(S\) limit^{53} and the large\(N\) limit.^{54} In doing so, it provides an unbiased analysis of the competition between magnetic ordering and disordering tendencies.^{27,51,52,53}
The flow equations are numerically solved in direct space and, after the Fourier transform of the spin–spin correlations, one obtains the static susceptibility in reciprocal space \(S({\bf{q}})\) as a function of \(\Lambda\). Note that the RG parameter \(\Lambda\) can be interpreted as the temperature \(T\)^{27} and is therefore used as a proxy to investigate the thermal evolution of the magnetic response. In the present study, we evaluate spin correlators within a cube of edge length of \(5a\), where \(a\) is the cubic lattice constant, which incorporates a total of 2315 correlated sites, producing wellconverged results with a high \({\bf{q}}\)space resolution. Furthermore, we approximate the frequency dependence of the vertex functions by discrete grids containing 64 points for each frequency variable. An ordered system is identified by cusps or kinks in the susceptibility flow signaling a magnetic instability towards either magnetic or valence bond order.^{51} In contrast, a smooth flow of the susceptibility down to \(\Lambda \to 0\) indicates a magnetically disordered state, that is, a putative (quantum) spin liquid.^{51}
Luttinger–Tisza method
In the Luttinger–Tisza method^{55,56,57} the ground state and energy spectrum of a classical spin system are approximately calculated. The classical limit of Eq. (1) consists of replacing the spin operators by classical vectors, which are normalized (the so called strong constraint). To find an approximate ground state, this constraint is relaxed to be fulfilled only on average over the whole system. This allows to Fourier transform the interaction matrix \({J}_{ij}\) with respect to the underlying Bravais lattice of the actual spin lattice, leading to a matrix \({J}_{\alpha \beta }({\bf{k}})\), where \(\alpha ,\beta\) label the basis points of the lattice.
The eigenvalues \(\lambda ({\bf{k}})\) of this matrix subsequently give the energies of spin spiral states with wave vector \({\bf{k}}\), the aforementioned energy spectrum, and the absolute value of the corresponding eigenvector components give the relative length of the vector spins on the different basis points. This means, that for such a state to fulfill the strong constraint, all components have to have equal absolute value.
If the lattice is of Bravais type, there is only one basis point and therefore the Fourier transformed interaction matrix is a scalar, which means this condition is trivially fulfilled, rendering the Luttinger–Tisza method exact on such lattices. In this case, we can also, through the equivalence of the Luttinger–Tisza method and PFFRG for \(S\to \infty\),^{53} calculate the classical spin susceptibility
Iterative minimization method
By employing the iterative minimization method,^{27,57} we find the ground state of the classical version of Eq. (1) obtained by replacing the spin operators by normalized vectors. In this scheme, we typically start from a random spin configuration, randomly select one vectorspin \({{\bf{S}}}_{i}\) at a time and rotate it to make it antiparallel to its local field
thus minimizing the energy. In a given sweep, we update all the spins contained in the configuration so that on average each spin is updated once. For our calculations, we use 32 cubic unit cells of the pyrochlore lattice in each direction with periodic boundary conditions, totaling to \(16\times 3{2}^{3}=524,288\) spins in the system. Convergence is reached once the total energy difference per sweep is <\(1{0}^{10}\) K. To reduce the likelihood of the system getting stuck at a local energy minimum in configuration space, we carry out the minimization for at least 20 different random initial configurations. We also use specific nonrandom configurations, e.g. spin spirals, as a starting point, to test exact spin parameterizations and, possibly, find lower minimal energies than those achieved by starting with arbitrary random spin configurations.
CMC method
We have performed CMC simulations for the model Hamiltonian parameters of the compounds as obtained from DFT given in Table 1, employing the standard single spinflip technique. For each Monte Carlo update, we perform the Metropolis moves as many times as the number of spins in the configuration such that, on average, each spin is updated once. Starting from a random spin configuration and after allowing for the system to reach thermal equilibrium, we evaluate the Fourier transform of the equaltime spin–spin correlator, i.e., the static structure factor \(S({\bf{q}})\) for 50 different configurations where each configuration is separated by 100 Monte Carlo updates. At lower temperatures, in order to increase the number of accepted moves, we restrict the newly generated spins to a small cone around its predecessor. The simulations are done for a system of \(32\times 32\times 32\) cubic unit cells of the pyrochlore lattice with periodic boundary conditions in each direction, amounting to \(16\times 3{2}^{3}\) spins. The entire simulations are independently carried out 15 times and the average of the results is taken for suppression of numerical noise.
Data availability
All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Materials. Additional data related to this paper may be requested from the authors.
References
Lacroix, C., Mendels, P., & Mila, F. Introduction to Frustrated Magnetism, Springer Series in SolidState Sciences (Springer, Heidelberg, 2011).
Gardner, J. S., Gingras, M. J. P. & Greedan, J. E. Magnetic pyrochlore oxides. Rev. Mod. Phys. 82, 53–107 (2010).
Hallas, A. M., Gaudet, J. & Gaulin, B. D. Experimental insights into groundstate selection of quantum XY pyrochlores. Annu. Rev. Condens. Matter Phys. 9, 105–124 (2018).
Rau, J. G. & Gingras, M. J. P. Frustrated quantum rareearth pyrochlores. Annu. Rev. Condens. Matter Phys. 10, 357–386 (2019).
Plumb, K. W. et al. Continuum of quantum fluctuations in a threedimensional \(S=1\) Heisenberg magnet. Nat. Phys. 15, 54–59 (2019).
Okamoto, Y., Nilsen, G. J., Attfield, J. P. & Hiroi, Z. Breathing pyrochlore lattice realized in Asite ordered spinel oxides LiGaCr\({}_{4}\)O\({}_{8}\) and LiInCr\({}_{4}\)O\({}_{8}\). Phys. Rev. Lett. 110, 097203 (2013).
Duda, H. et al. Spinglasslike behavior in singlecrystalline Cu\({}_{0.44}\)In\({}_{0.48}\)Cr\({}_{1.95}\)Se\({}_{4}\). Phys. Rev. B. 77, 035207 (2008).
Tanaka, Y., Yoshida, M., Takigawa, M., Okamoto, Y. & Hiroi, Z. Novel phase transitions in the breathing pyrochlore Lattice: \({}^{7}\)LiNMR on LiInCr\({}_{4}\)O\({}_{8}\) and LiGaCr\({}_{4}\)O\({}_{8}\). Phys. Rev. Lett. 113, 227204 (2014).
Nilsen, G. J. et al. Complex magnetostructural order in the frustrated spinel LiInCr\({}_{4}\)O\({}_{8}\). Phys. Rev. B. 91, 174435 (2015).
Okamoto, Y., Nilsen, G. J., Nakazono, T. & Hiroi, Z. Magnetic phase diagram of the breathing pyrochlore antiferromagnet LiGa\({}_{1x}\)In\({}_{x}\)Cr\({}_{4}\)O\({}_{8}\). J. Phys. Soc. Jpn. 84, 043707 (2015).
Lee, S. et al. Multistage symmetry breaking in the breathing pyrochlore lattice Li(Ga,In)Cr\({}_{4}\)O\({}_{8}\). Phys. Rev. B. 93, 174402 (2016).
Saha, R. et al. Magnetodielectric effects in Asite cationordered chromate spinels Li\(M\)Cr\({}_{4}\)O\({}_{8}\) (\(M\) = Ga and In). Phys. Rev. B. 94, 064420 (2016).
Okamoto, Y. et al. Magnetic transitions under ultrahigh magnetic fields of up to 130 T in the breathing pyrochlore antiferromagnet LiInCr\({}_{4}\)O\({}_{8}\). Phys. Rev. B. 95, 134438 (2017).
Wawrzyńczak, R. Classical spin nematic transition in LiGa\({}_{0.95}\)In\({}_{0.05}\)Cr\({}_{4}\)O\({}_{8}\). Phys. Rev. Lett. 119, 087201 (2017).
Pokharel, G. et al. Negative thermal expansion and magnetoelastic coupling in the breathing pyrochlore lattice material LiGaCr\({}_{4}\)S\({}_{8}\). Phys. Rev. B. 97, 134117 (2018).
Okamoto, Y. Magnetic and structural properties of Asite ordered chromium spinel sulfides: alternating antiferromagnetic and ferromagnetic interactions in the breathing pyrochlore lattice. J. Phys. Soc. Jpn. 87, 034709 (2018).
Joubert, J.C. & Durif, A. Étude de quelques composés spinelles nouveaux possédant un ordre des cations du type 1/1 sur les sites tétraédriques. Bull. Soc. Fr. Mineral. Cristallogr. 89, 26–28 (1966).
Benton, O. & Shannon, N. Ground state selection and spinliquid behaviour in the classical Heisenberg model on the breathing pyrochlore lattice. J. Phys. Soc. Jpn. 84, 104710 (2015).
Tsunetsugu, H. Theory of antiferromagnetic Heisenberg spins on a breathing pyrochlore lattice. Prog. Theor. Exp. Phys. 2017, 033I01 (2017).
Aoyama, K. & Kawamura, H. Spin ordering induced by lattice distortions in classical Heisenberg antiferromagnets on the breathing pyrochlore lattice. Phys. Rev. B. 99, 144406 (2019).
Li, F.Y. et al. Weyl magnons in breathing pyrochlore antiferromagnets. Nat. Commun. 7, 12691 (2016).
Ezawa, M. Higherorder topological insulators and semimetals on the breathing kagome and pyrochlore lattices. Phys. Rev. Lett. 120, 026801 (2018).
Moessner, R. & Chalker, J. T. Properties of a classical spin liquid: the Heisenberg pyrochlore antiferromagnet. Phys. Rev. Lett. 80, 2929–2932 (1998).
Bergman, D., Alicea, J., Gull, E., Trebst, S. & Balents, L. Order by disorder and spiral spin liquid in frustrated diamond lattice antiferromagnets. Nat. Phys. 3, 487–491 (2007).
Iqbal, Y. et al. Signatures of a gearwheel quantum spin liquid in a spin1/2 pyrochlore molybdate Heisenberg antiferromagnet. Phys. Rev. Mater. 1, 071201(R) (2017).
Tapp, J. et al. From magnetic order to spinliquid ground states on the \(S=3/2\) triangular lattice. Phys. Rev. B. 96, 064404 (2017).
Iqbal, Y. et al. Quantum and classical phases of the pyrochlore Heisenberg model with competing interactions. Phys. Rev. X. 9, 011005 (2019).
Conlon, P. H. & Chalker, J. T. Absent pinch points and emergent clusters: further neighbor interactions in the pyrochlore Heisenberg antiferromagnet. Phys. Rev. B. 81, 224413 (2010).
Chern, G.W., Moessner, R. & Tchernyshyov, O. Partial order from disorder in a classical pyrochlore antiferromagnet. Phys. Rev. B. 78, 144418 (2008).
Iqbal, Y., Thomale, R., Toldin, F. P., Rachel, S. & Reuther, J. Functional renormalization group for threedimensional quantum magnetism. Phys. Rev. B. 94, 140408(R) (2016).
Iqbal, Y., Müller, T., Jeschke, H. O., Thomale, R. & Reuther, J. Stability of the spiral spin liquid in MnSc\({}_{2}\)S\({}_{4}\). Phys. Rev. B. 98, 064427 (2018).
Rück, M. & Reuther, J. Effects of twoloop contributions in the pseudofermion functional renormalization group method for quantum spin systems. Phys. Rev. B. 97, 144404 (2018).
Kugler, F. B. & von Delft, J. Multiloop functional renormalization group that sums up all parquet diagrams. Phys. Rev. Lett. 120, 057403 (2018).
Brown, P. J., Fox, A. G., Maslen, E. N., O ’ Keefe, M. A. & Willis, B. T. M. in International Tables for Crystallography, Vol. C: Mathematical, Physical and Chemical Tables (ed. Prince, E.) 454–460 (Springer Netherlands, Dordrecht, 2004).
Kimchi, I. & Vishwanath, A. Kitaev–Heisenberg models for iridates on the triangular, hyperkagome, kagome, fcc & pyrochlore lattices. Phys. Rev. B. 89, 014414 (2014).
Henley, C. L. Ordering by disorder: ground state selection in fcc vector antiferromagnets. J. Appl. Phys. 61, 3962–3964 (1987).
Oguchi, T., Nishimori, H. & Taguchi, Y. The spin wave theory in antiferromagnetic Heisenberg model on face centered cubic lattice. J. Phys. Soc. Jpn. 54, 4494–4497 (1985).
Plumier, R., Lotgering, F. K. & van Stapele, R. P. Magnetic properties of Cu_{1/2}In_{1/2}Cr_{2}S_{4} and some related compounds. J. Phys. Colloq. 32, C1 324–C1 325 (1971).
Plumier, R., Sougi, M. & Lecomte, M. Observation of an unusual short range magnetic ordering in spinel Cu\({}_{1/2}\)In\({}_{1/2}\)Cr\({}_{2}\)S\({}_{4}\). Phys. Lett. 60A, 341–344 (1977).
Tymoshenko, Y. V. et al. PseudoGoldstone magnons in the frustrated \(S=3/2\) Heisenberg helimagnet ZnCr\({}_{2}\)Se\({}_{4}\) with a pyrochlore magnetic sublattice. Phys. Rev. X. 7, 041049 (2017).
Bai, X. et al. Magnetic excitations of the classical spin liquid MgCr\({}_{2}\)O\({}_{4}\). Phys. Rev. Lett. 122, 097201 (2019).
Gao, S. et al. Spiral spinliquid and the emergence of a vortexlike state in MnSc\({}_{2}\)S\({}_{4}\). Nat. Phys. 13, 157–161 (2016).
Haeuseler, H. & Lutz, H. D. Gitterschwingungsspektren XVIII. Chromthio und Chromselenospinelle mit 1:1Ordnung auf den Tetraederplätzen. J. Solid State Chem. 22, 201–204 (1977).
Koepernik, K. & Eschrig, H. Fullpotential nonorthogonal localorbital minimumbasis bandstructure scheme. Phys. Rev. B. 59, 1743–1757 (1999).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).
Liechtenstein, A. I., Anisimov, V. I. & Zaanen, J. Densityfunctional theory and strong interactions: orbital ordering in Mott–Hubbard insulators. Phys. Rev. B. 52, R5467–R5470 (1995).
Mizokawa, T. & Fujimori, A. Electronic structure and orbital ordering in perovskitetype \(3d\) transitionmetal oxides studied by Hartree–Fock bandstructure calculations. Phys. Rev. B. 54, 5368–5380 (1996).
Jeschke, H. O. et al. Multistep approach to microscopic models for frustrated quantum magnets: the case of the natural mineral azurite. Phys. Rev. Lett. 106, 217201 (2011).
Iqbal, Y. et al. Paramagnetism in the kagome compounds (Zn,Mg,Cd)Cu\({}_{3}\)(OH)\({}_{6}\)Cl\({}_{2}\). Phys. Rev. B. 92, 220404(R) (2015).
Guterding, D., Valentí, R. & Jeschke, H. O. Reduction of magnetic interlayer coupling in barlowite through isoelectronic substitution. Phys. Rev. B. 94, 125136 (2016).
Reuther, J. & Wölfle, P. \({J}_{1}\)\({J}_{2}\) frustrated twodimensional Heisenberg model: random phase approximation and functional renormalization group. Phys. Rev. B. 81, 144410 (2010).
Metzner, W., Salmhofer, M., Honerkamp, C., Meden, V. & Schönhammer, K. Functional renormalization group approach to correlated fermion systems. Rev. Mod. Phys. 84, 299–352 (2012).
Baez, M. L. & Reuther, J. Numerical treatment of spin systems with unrestricted spin length \(S\): a functional renormalization group study. Phys. Rev. B. 96, 045144 (2017).
Buessen, F. L., Roscher, D., Diehl, S. & Trebst, S. Functional renormalization group approach to \(SU(N)\) Heisenberg models: realspace renormalization group at arbitrary \(N\). Phys. Rev. B. 97, 064415 (2018).
Luttinger, J. M. & Tisza, L. Theory of dipole interaction in crystals. Phys. Rev. 70, 954–964 (1946).
Kaplan, T. A. & Menyuk, N. Spin ordering in threedimensional crystals with strong competing exchange interactions. Phil. Mag. 87, 3711–3785 (2007).
Lapa, M. F. & Henley, C. L. Ground states of the classical antiferromagnet on the pyrochlore lattice. Preprint at https://arxiv.org/abs/1210.6810 (2012).
Acknowledgments
We thank Zenji Hiroi, Gøran Nilsen, Yoshihiko Okamoto, Owen Benton, Hikaru Kawamura, and Jason Gardner for useful discussions. H.O.J. thanks Gøran Nilsen for communicating the \(T=20\) K internal coordinates of LiInCr_{4}O_{8}. We gratefully acknowledge the Gauss Centre for Supercomputing e.V. for funding this project by providing computing time on the GCS Supercomputer SuperMUC at Leibniz Supercomputing Centre (LRZ). The work in Würzburg is funded by the Deutsche Forschungsgemeinschaft (DFG, German Research Foundation)ProjectID 258499086SFB 1170 and by the WürzburgDresden Cluster of Excellence on Complexity and Topology in Quantum Matter—ct.qmat (EXC 2147, projectid 39085490). This research was supported in part by the International Centre for Theoretical Sciences (ICTS) during a visit for participating in the program—The 2nd Asia Pacific Workshop on Quantum Magnetism (Code: ICTS/apfm2018/11). J.R. acknowledges the kind hospitality of the Indian Institute of Technology Madras, Chennai, India, where a part of the research was carried out. The work at the University of Waterloo was supported by the Canada Research Chair program (M.J.P.G., Tier 1).
Author information
Authors and Affiliations
Contributions
H.O.J. initiated the project. P.G., Y.I., T.M., J.R., R.T.P. and H.O.J. performed the calculations. All authors analyzed the data and contributed to their interpretation. P.G., Y.I., M.J.P.G. and H.O.J. wrote the manuscript with input from all authors.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Ghosh, P., Iqbal, Y., Müller, T. et al. Breathing chromium spinels: a showcase for a variety of pyrochlore Heisenberg Hamiltonians. npj Quantum Mater. 4, 63 (2019). https://doi.org/10.1038/s415350190202z
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s415350190202z
This article is cited by

Towards understanding the magnetic properties of the breathing pyrochlore compound Ba3Yb2Zn5O11through singlecrystal studies
npj Quantum Materials (2022)

Fieldtunable toroidal moment in a chirallattice magnet
Nature Communications (2021)